Cerium molybdate nanocrystals: Microstructural, optical and gas-sensing properties

.


Introduction
Metallic molybdates have aroused interest in several sectors of the industry due to their potential applications in different areas, such as photoluminescence, photocatalysis, and gas sensors [1e7].In the case of gas-sensing devices, the automotive industry performs daily diverse industrial processes which involve the combustion of fossil fuels, consequently generating several pollutants, such as O 3 , CO, NO x , NH 3 , and SO 2 [8,9].In the lower atmosphere, these harmful gases cause damage to the environment as well as to human health [10].
Among the harmful pollutants, ozone (O 3 ) is a strong oxidizing agent used in several practical applications in food industry, water drinking treatment and medical therapies, etc [11e13].It is formed in the troposphere as a result of photochemical reactions, being related to the pollution generated by vehicles and industrial processes.However, high O 3 gas levels are currently being monitored because of the congestion and inflammation processes which occur when in contact with the human respiratory system [14e16].To solve this problem, analytical techniques have been used to measure O 3 levels in the range of 0.01e10 ppm (parts per million), which are extremely necessary for industrial sensors [17,18].These concentrations are required to be detected precisely and rapidly.
Resistive gas sensors are composed of a sensing layer made by semiconducting metal oxide (MOX) or multi-metal oxide (MMO) materials [19,20].MOXs have been widely studied due to its simple structure, low cost, and abundance.There are several MOXs described in the literature with potential applications as sensing layers, meanwhile the main MOX used as sensing material in chemical gas sensor devices are SnO 2 [21], ZnO [22], WO 3 [23], In 2 O 3 [24], and CuO [25].These MOXs have presented high sensitivity for different analytes (reducing and oxidizing), good stability, and low production cost, facilitating their integration into sensor devices [8,26,27].As mentioned, MMO nanomaterials (such as NaBi(MoO 4 ) 2 ) are another class of materials currently used to improve gas detection because of their adjustable structural, photocatalytic, catalytic, and electrical properties [28].On the other hand, few papers investigate the gas-sensing performance of MMOs compounds [3,4].
Among the MMOs, we can highlight A 2 (MoO 4 ) 3 molybdates, which belong to the scheelite family and can have tetragonal or monoclinic structures, where A atoms can be La 3þ , Ce 3þ , Pr 3þ , Nd 3þ , Sm 3þ and Eu 3þ [29].These types of structures can promote complex molybdates and provide high feasibility for incorporating different doping metals, including rare-earth elements [30].Therefore, rareearth metal(III) exhibits a tetragonal structure with space group I4 1 / a, in which the [MoO 4 ] cluster is coordinated by four oxygen atoms resulting in a polyhedral which can be strongly distorted [31e34] metallic clusters without complete occupancy.Ce 2 (MoO 4 ) 3 nanocrystals are inorganic materials that have received great attention due to their photoluminescent [34], biosensing [35], photonic [34] and catalytic [36,37] properties, having application in various fields.Several synthesis methods have been used to produce Ce 2 (MoO 4 ) 3 nanocrystals, such as organometallic precursors [32], sol-gel [38], and solvothermal [33] and microwaveassisted hydrothermal/solvothermal methods [34].Singh et al. synthesized cerium molybdate by the hydrothermal method at 180 C for different times (from 6 to 48 h), using a mixture of water and ethanol as synthesis solvents to obtain the pure phase [35].In contrast, Maisang et al. synthesized cerium molybdate by the microwave-assisted hydro/solvothermal method and obtained the monoclinic phase [34].
In the present study, we describe the synthesis of Ce 2 (MoO 4 ) 3 nanocrystals via a microwave-assisted route and their structural, optical, and gas-sensing properties.To the best of our knowledge, this is the first time that cerium molybdate is used as a sensing material for the detection of sub-ppm ozone levels.The nanocrystals were obtained by the co-precipitation method and then treated in a microwave-assisted hydrothermal (MAH) system at 150 C for different times (15, 30, and 60 min).The as-obtained Ce 2 (MoO 4 ) 3 nanocrystals were investigated by X-ray diffraction, micro-Raman spectroscopy, ultravioletevisible spectroscopy, electron microscopies (FEG-SEM and HRTEM), and photoluminescent (PL) measurements.Gas-sensing experiments revealed good sensitivity and repeatability as well as total recovery after consecutive exposures to various O 3 gas levels.in 50 mL of distilled water.The solution pH was adjusted to 7 by adding a strong base to increase the hydrolysis rate.The resulting solution was stirred for 30 min.Afterwards, the mixture was transferred to a Teflon reactor and processed by a microwaveassisted hydrothermal system (2.45 GHz, maximum power of 800 W).The microwave-assisted hydrothermal processing was performed at 150 C for different times: 15, 30, and 60 min.The asprepared samples were labeled as CeMO15, CeMO30, and CeMO60, respectively.After the microwave-assisted hydrothermal treatment, the solution was naturally cooled down to room temperature.Then, it was washed with distilled water and ethanol several times.Finally, the yellow powders were collected and dried at 100 C for 24 h.

Characterizations of Ce 2 (MoO 4 ) 3 powders
Ce 2 (MoO 4 ) 3 nanocrystals were structurally characterized by Xray diffraction using a diffractometer (Shimadzu, XRD-7000, with Cu-Ka radiation) in the 2q range from 10 to 80 and with a step size of 0.02 /min.The morphological properties and particle size were investigated using field-emission gun scanning electron microscopy (FEG-SEM) (Supra 35-VP, Carl Zeiss, Germany) operated at different magnifications.Transmission electron microscopy (TEM), high-resolution transmission electron microscopy (HRTEM) images, and chemical analysis using energy-dispersive X-ray spectroscopy (EDS) were performed with a FEI TECNAI G2 F20 microscope operating at 200 kV.
Raman measurements were recorded at room temperature using a T-64000 (Jobin-Yvon, France) triple monochromator coupled to a CCD detector.UVevis absorption spectra were achieved using a UV-2600 (Shimadzu) device in total reflectance mode.Room-temperature photoluminescence (PL) spectra were collected with an ANDOR-Kymera 193i-B1 device using a 355 nm line of a krypton ion laser (Coherent Innova 90 K, USA) in a Mosospec 27 monochromator and a photomultiplier (Hamamatsu R446).

Gas-sensing measurements
The as-obtained Ce 2 (MoO 4 ) 3 samples were dispersed in isopropyl alcohol by an ultrasonic cleaner for 30 min.The suspension was then dripped onto a pre-cleaned Al 2 O 3 substrate with interdigitated Pt electrodes [39].Afterwards, the samples were annealed at 500 C for 30 min in an electric oven under air atmosphere.The sensor samples were then inserted into a dynamic chamber that allows the control of the operating temperature (up to 350 C) and the O 3 gas levels by using mass flow controllers (MFC).Further details regarding the gas-sensing workbench may be found in a previous work [23].Ozone gas was formed from oxidizing oxygen molecules of dry air by a calibrated pen-ray UV lamp (UVP, model P/ N 90-0004-01), which provided concentrations from 0.07 to 0.53 ppm that were verified using a toxic gas detector (ATI, model F12).The total gas flow rate was kept constant at 500 SCCM (Standard Cubic Centimeters per Minute).The applied DC voltage was also kept constant, while the electrical resistance was monitored using an electrometer (Keithley, model 6514).The sensor response (S) was defined as S ¼ R air /R O3 , where R air and R O3 are the electric resistances of the device exposed to dry air and gas, respectively.synthesized by unequal methods were obtained with the presence of monoclinic phase [32], hydrate form [33], or secondary phases, such as Ce(OH) [34], Ce 11 O 20 and Ce 7 O 12 [31], which is in accordance with the literature.The analysis of these results reveals that the preparation of nanocrystals by the MAH method can promote the obtention of the pristine Ce 2 (MoO 4 ) 3 phase, even at shorter MAH times.

Structural analyses
The lattice parameters and unit cell volume were calculated using the General Structure Analysis System (GSAS) with an EXPGUI graphic interface [41] to obtain quantified information regarding the influence of MAH time on the structural properties of Ce 2 (MoO 4 ) 3 nanocrystals.Further information on Ce 2 (MoO 4 ) 3 nanocrystals was investigated by the Rietveld refinement method using the Inorganic Crystal Structure Database (ICSD) card No. 423509 [40].These results (Table 1 and Fig. S1) demonstrate the high quality of the refinements with regard to the lattice parameters, cell volume, refinement reliability parameters, and crystalline size, while the microstrain was revealed by statistical fitting parameters (R p , RF 2 , and c 2 ) [42].
The refinement results confirm that the Ce 2 (MoO 4 ) 3 nanocrystals obtained by the MAH method present a pure tetragonal phase with I41/a space group.Additionally, the obtained results of the lattice parameters and unit cell of Ce 2 (MoO 4 ) 3 nanocrytals are in good agreement with the data reported in the ICSD card No. 423509, as shown in Table 1.Nevertheless, some variations in such parameters were observed when comparing the Ce 2 (MoO 4 ) 3 samples processed by the MAH route and the reference data (ICSD card no.423509), which can be linked to different types of synthesis methods [40].Regarding the MAH time, we noted variations in the values of the lattice parameters a and c, i.e., a reduction in the parameter a and an increase in the parameter c as a function of MAH time, which implies the stretching of the tetragonal structure indicated by the c/a ratio.Likewise, the amount of phase crystallinity and the average crystallite size were also influenced by the MAH time, as seen in Table 1.processing and treatment time [44].
On the other hand, the site of the Ce 3þ cations cannot be fully occupied in this structure due to the need to maintain the electroneutrality conditions.Because of this, two-thirds of the Ce atoms are coordinated to eight oxygen atoms and two CeeO bond paths, thus forming trigonal dodecahedral [Ce 0$667 O 8 ] clusters [40,45e47].Similar to the MoeO bond path, the CeeO bond path exhibited a small difference between the samples CeMO15 (CeeO ¼ 2.553 Å (4x) and 2.597 Å (4x)) and CeMO30 (CeeO ¼ 2.533 Å (4x) and 2.581 Å (4x)), while the CeMO60 nanocrystals presented a more expressive distortion (CeeO ¼ 2.522 Å (4x) and 2.693 Å (4x)).Therefore, the Ce 2 (MoO 4 ) 3 sample obtained by the MAH route proved to be extremely sensitive to the synthesis time.In addition, since such structural modifications are strongly influenced by the cluster distortions, they can usually result in improved properties [48].

Raman spectroscopy
The Raman-active phonon modes are a powerful characterization to investigate and estimate the short-range structural order in the materials [49].According to the literature [50,51], the scheelitetype tetragonal structure has 26 different modes in the theoretical calculation (G ) for zero wavevectors of the scheelite primitive cell, where 13 vibration modes (3A g , 5B g, and 5E g ) are active in the Raman spectra, while only 8 (4A u and 4E u ) are active in the infrared.In contrast, 2 modes (A u and E u ) are acoustic vibrations and the 3B u vibrations are silent modes.
According to Raman spectroscopy, there are only two vibrational modes in scheelite structures, namely external and internal modes [50,52].The first corresponds to the motion of the Ce 3þ cation and the rigid [MoO 4 ] 2À tetrahedral molecular units, while the second, considered as the stationary state of the mass center, belongs to the vibration inside [MoO 4 ] 2À tetrahedral units [46,53].The [MoO 4 ] 2¡ tetrahedrons have T d symmetry in free space [50], and their internal modes are composed by n 1 (A 1 ), n 2 (E 1 ), n 3 (F 2 ) and n 4 (F 2 ), one free rotation mode, n fr , (F 1 ) and one translation mode (F 2 ) [54].
Fig. 3 displays the Raman spectra of the Ce 2 (MoO 4 ) 3 nanocrystals in the range of 100 to 1200 cm À1 .The spectra clearly show the existence of three bands at 893, 380, and 316 cm À1 .In addition, we can observe shifts in the Raman modes of Ce 2 (MoO 4 ) 3 caused by the covalent bond formation between Mo 6þ and O 2À ions in the [MoO 4 ] clusters, which change the efficient mass of the oscillating atoms.This phenomenon can be influenced by some parameters, such as preparation methodology, average crystal size, distortions in the OeMoeO and OeCeeO bonds, interaction forces between the ions, or even the degree of structural order in the lattice [55].
The active Raman modes show that the Ce 2 (MoO 4 ) 3 nanocrystals are structurally disordered at short range.The analysis of the results reveals the presence of n 1 (A g ) mode at approximately 893 cm À1 , which is associated with the symmetric stretching of the tetrahedral [MoO 4 ] clusters.The peaks at 824 and 795 cm À1 corresponding to n 3 (B g ) and n 3 (E g ) modes, respectively, are attributed to the anti-symmetric stretching.At 380 cm À1 , a less intense n 4 (B g ) mode is identified, and the peak at 316 cm À1 is a stronger n 2 (A g ) mode of the regular [MoO 4 ] cluster [56].Regarding the MAH time, we also observed an increase in the intensity of the modes as a function of MAH treatment time (Fig. 3), revealing an enhancement of structural organization of the Ce 2 (MoO 4 ) 3 samples, which is in good agreement with the XRD analyses.plates, in addition to presenting a polydispersal nature with a random growing without orientation planes.Fig. 4(d-i) reveal that the samples CeMO30 and CeMO60 are formed by nanoplate and polyhedron-shaped morphology with larger particle sizes when compared to CeMO15, which has a relationship with the crystallite size values seen in Table 1.The morphology of the CeMO30 and CeMO60 nanocrystals had a similar shape to that reported by Singh et al. [35] when they synthesized Ce 2 (MoO 4 ) 3 at 180 C for 48 h via the conventional hydrothermal route.Therefore, this morphology tends to be formed in hydrothermal methods in the absence of surfactants.
The morphological variations found in Ce 2 (MoO 4 ) 3 nanocrystals can be attributed to the microwave radiation used in the MAH method, which promotes high heating rates, many collisions of atoms, and fast formation of nanoparticles present in the Ce 2 (MoO 4 ) 3 precursor solution.Both the MAH treatment time and heating provoke the nucleation of several crystalline nuclei due to microwave radiation penetration.Afterwards, when the nucleus reaches a critical size, it grows to form the particles so that a large number of particles prevents the overgrowth of the others [2,57].The MAH method also allows the obtention of crystalline compounds in short synthesis times compared to the conventional hydrothermal route.Since the increase in the synthesis time allowed particle growth and morphology changes, all the events aforementioned can justify the adsorption process between the particles [58e60].
Fig. 5 (a-f) display the TEM images of the as-obtained samples CeMO15, CeMO30, and CeMO60.It is possible to observe that the CeMO15 particles are quite thin as a nanosheet on account of their high TEM beam transmittance, resulting in images with translucent particles.However, longer MAH synthesis times promoted the growth of thicker particles due to a lower TEM beam transmittance, consequently enhancing the opacity of the particle image.Fig. 5 (g-i) show the HR-TEM images of the nanocrystals, where it is possible to see interplanar distances of 0.32, 0.31, and 0.31 nm for CeMO15, CeMO30, and CeMO60, respectively, which correspond to the (112) Miller index.Furthermore, the SAED patterns in Fig. 5 (j-l) confirm the polycrystalline nature of the as-obtained materials, demonstrated by the diffraction concentric rings of (112), (002), (024), and (116) planes, which could be observed according to their interplanar spacing in the respective figures and Table 2.The SAED patterns proved that Ce 2 (MoO 4 ) 3 nanocrystals were formed.
EDS analysis was used for the elemental characterization of the Ce 2 (MoO 4 ) 3 nanocrystals.Fig. 6(aec) indicate the presence of the elements O, Ce, and Mo as well as the elements C, Ni, and Cu from the TEM grid.

UVevis absorption spectroscopy analyses
The optical gap (E gap ) was first estimated from the diffuse reflectance data and converted to absorbance through the Kubelka-Munk function [61e63], then calculated by the method proposed by Wood and Tauc [64].Fig. 7 shows the band gap energy for all Ce 2 (MoO 4 ) 3 samples, using n ¼ 1/2 (i.e.direct permissible transition) [32,34].Each energy gap was determined by extrapolating each linear portion of the curves until a ¼ 0. According to our study, the increase of the MAH time was not able to promote the formation of intermediate energy levels between the valence (VB) and conduction (CB) bands in Ce 2 (MoO 4 ) 3 nanocrystals.Moreover, the presence of these energy levels was found to be dependent on the degree of structural order-disorder in the lattice [44].
As a result, we could observe that the E gap value ranged between 2.76 and 2.84 eV, which is consistent with the values reported in the literature for the Ce 2 (MoO 4 ) 3 compound [32,34].These values can then indicate that the samples present a certain degree of order-disorder, which directly influences their structural defects.The result of the PL spectra indicates that all Ce 2 (MoO 4 ) 3 nanocrystals exhibit broadband emission with maximum intensity at approximately 500 nm (blue-green region).This behavior can be explained by the multiphonon and multilevel process, where the relaxation process involves many states that participate in several levels within the band gap of the material [65,66].

Photoluminescence analyses
Several studies in the literature have reported on the possible origin of the PL properties of molybdates, basing their explanations on the recombination of electrons in the 1 T 2 excited state and holes in the 1 A 1 ground state [67], the charge transfer transitions within the [MoO 4 ] 2-complex [68], the energy absorption of the 2p orbitals of oxygen and the promotion of molybdenum 4d orbital [69], and vacancies in the oxygen complex [MoO 4 ] clusters [70].
Fig. 8 (a) indicates that the maximum PL emission of the Ce 2 (MoO 4 ) 3 nanocrystals are in the blue region and centered around 463, 474, and 483 nm for CeMO15, CeMO30, and CeMO60, respectively, which is generally attributed to a charge diffusion from the Ce 4f level to the O 2p level [71].As previously mentioned, several authors have tried to determine the mechanism of the PL properties.Using theoretical investigations, our group has proposed that the physical property is directly associated with distortions in the [MoO 4 ] and [XO 8 ] clusters (X ¼ Ca, Ba, Pb, Sr) [72].Therefore, in our study we could observe a substantial increase in the intensity of the PL emission with MAH time.This finding can be related to the degree of order-disorder of the nanocrystals as a function of MAH time, which consequently generated defects that induced symmetry breaking in the material.However, some studies have attributed the increase in the PL spectra to a slightly intrinsic distortion of the tetrahedral [MoO 4 ] clusters, the morphology, and the charge-transfer transitions within the [MoO 4 ] 2-complex (ions) [45,70,73e75].These distortions are responsible, for example, for the excellent interaction between the Mo atoms and the microwave radiation, and the continuous dissolution and recrystallization mechanisms during the crystal growth processes.
As it can be seen in Fig. 2 S1).

Ozone gas-sensing performance
As previously mentioned, few studies have focused on the gassensing performance of molybdates.In one of them, Zou et al. reported the gas-sensing properties of a composite based on Fe 2 (MoO 4 ) 3 microspheres for the detection of butanol [4].With regard to the sensitivity towards ozone (O 3 ) gas, at the present moment we have not found any study in the literature, justifying our investigation on the ozone gas-sensing properties of Ce 2 (MoO 4 ) 3 nanocrystals.
The thermal stability of the tetragonal phase of the powders was measured by thermal treatment at 500 C for 30 min, and the conservation of such phase after thermal treatment was observed, as it can be seen in Figure S2.The optimum operating temperature (T opt ) of the Ce 2 (MoO 4 ) 3 nanocrystals was initially investigated by varying the T opt from 100 to 350 C and exposing each sample to  0.07 ppm of O 3 gas for 30 s.According to Fig. 9, the sensor responses increase with the operating temperature (T opt ), reaching a maximum value at approximately 200 C, and then decrease at higher temperatures.This behavior was identified in both samples (CeMO30 and CeMO60); however, the latter exhibited a higher response at this temperature than the first.This enhancement can be attributed to the presence of additional active sites on the CeMO60 surface, possibly formed as a result of longer MAH synthesis time.We would like to draw attention to the following points: (i) due to the high resistance of the samples, the lowest T opt studied was 100 C; (ii) the sample CeMO15 did not exhibit any sensitivity towards different O 3 levels, considering the T opt and the gas level range investigated herein.
According to the literature, the traditional MOXs used as ozone sensing layer are SnO 2 , ZnO, WO 3 , and In 2 O 3 [13,76,77].These MOXs have been treated at temperatures of around 150 and 300 C. Thus, the working temperature obtained herein for cerium molybdate samples demonstrates its potential as an O 3 sensing layer.
The samples were kept at 200 C and then exposed to different gas levels (i.e. from 0.07 to 0.53 ppm) in order to investigate the O 3 detection range.As seen in Fig. 10 (a-b), the electrical resistance decreases under the presence of different O 3 levels, indicating a ptype conduction behavior [78,79].In addition, a gradual enhancement of the sensor response to O 3 concentration can be observed.It should be noted that both samples detected low ozone levels, even after consecutive exposure cycles, highlighting their complete recovery and chemical stability.
Furthermore, the response (t resp ) and recovery (t rec ) times for both samples were also estimated.The t resp is defined as the time required for the electrical resistance to reach 90% of the initial value when exposed to the analyte investigated, while t rec corresponds to the required time for the electrical resistance to reach 90% of its initial value after the interruption of the analyte flow.The obtained t resp values were similar for all samples, varying from 23 to 28 s (CeMO30) and 22e25 s (CeMO60) depending on the O 3 level investigated.On the other hand, CeMO30 presented a three times faster recovery than CeMO60, i.e. around 2 and 6 min, respectively.As abovementioned, the high sensitivity of CeMO60 implies a high density of O 3 molecules adsorbed, which require more time for their complete desorption from the sample surface.
Additionally, Fig. 10 shows that despite both samples successfully detected sub-ppm levels of O 3 gas, the sample CeMO60 exhibited a higher response, considering the O 3 levels investigated.
A brief summary of the T opt and the minimum O 3 level detected, recently reported for some MOXs synthesized by different methodologies, can be observed in Table 3.
As found in the literature, the superior sensing performance might be attributed to the presence of pre-adsorbed species on the semiconductor surfaces (acting as active sites), morphological features and the crystallization degree, among others [16,80e82].Therefore, our findings showed that the MAH treatment time plays an important role in the formation of active sites responsible for the adsorption of ozone molecules.We also observed similar improvements for the CuWO 4 compound annealed at different temperatures in conventional oven [61].

Conclusions
Ce 2 (MoO 4 ) 3 nanocrystals were synthesized by the coprecipitation method and treated at 150 C in a microwaveassisted hydrothermal system for 15, 30 and 60 min.According to the XRD and Raman results, the as-obtained nanocrystals presented a scheelite-type tetragonal structure without secondary phases.The FEG-SEM and TEM micrographs revealed the presence of crystals exhibiting nanosheet and nanoplate shapes.Regarding the optical properties, UVevis spectra showed that the optical band gap of cerium molybdates remained unchanged with MAH time.The PL spectrum of the sample CeMO60 (treated for 60 min) exhibited an intense broadband emission in the blue region, which was associated with oxygen vacancies and defects of [MoO 4 ] and/or [Ce 0$667 O 8 ] clusters formed during the MAH treatment.Electrical measurements revealed the ozone sensitivity of Ce 2 (MoO 4 ) 3 nanocrystals in the range of 0.07e0.53ppm.The samples presented a good response and total recovery after consecutive exposures, but mainly the one treated for 60 min (CeMO60).This behavior can be linked to the effect of the MAH treatment time, which favored the formation of active sites on the cerium molybdate surface.Finally, the promising properties of cerium molybdates synthesized via facile and clean route, the MAH method, make them potential candidates for application as sensing layer for the detection of subppm ozone levels.UFRN) and the Coordination of Improvement of Higher Education Personnel e CAPES (Finance Code 001).The electrodes used for the gas-sensing experiments were fabricated in the Laboratory of Microfabrication at the Brazilian Nanotechnology National Laboratory e LNNano/CNPEM (Project LMF-18580).The authors would also like to thank Prof. Maximo Lui for the photoluminescence measurements.

Fig. 1
Fig. 1 shows the XRD patterns of Ce 2 (MoO 4 ) 3 nanocrystals processed at different MAH treatment times.It was observed that all XRD reflections were indexed to the scheelite-type tetragonal structure following the Inorganic Crystal Structure Database (ICSD) card No. 423509 [40].In addition, the relative intensities and sharp peaks of the XRD measurements indicate that the Ce 2 (MoO 4 ) 3 nanocrystals are well crystallized, suggesting an ordered structure over a long range.Nevertheless, the Ce 2 (MoO 4 ) 3 compounds

Fig. 2
Fig. 2 illustrates a schematic representation of the Ce 2 (MoO 4 ) 3 tetragonal unit cell.This was modeled using the CrystalMaker

Fig. 8 (
Fig. 8 (a-b) show the room-temperature photoluminescence (PL) spectra and the CIE (International Commission on , the [MoO 4 ] clusters created greater distortions in a and b angles, which in turn caused the MoeO bond paths and OeMoeO angles to exhibit small variations between the samples CeMO15 (MoeO ¼ 1.711 Å (4x), a ¼ 108.6 , and b ¼ 112.3 ) and CeMO30 (MoeO ¼ 1.732 Å (4x), a ¼ 107.5 , and b ¼ 113.4 ), while the sample CeMO60 presented a larger distortion (MoeO ¼ 1.711 Å (4x), a ¼ 112.2 , and b ¼ 104.2 ).Such distortions in the Ce 2 (MoO 4 ) 3 nanoparticles are important for the formation of deep-level defect process and influence the blue PL emission more intensely in CeMO60 due to the longer time of exposure to microwave radiation.This observation was based on the structural refinement data performed for each Ce 2 (MoO 4 ) 3 nanocrystal (Fig. 2 and Table

Fig. 9 .
Fig. 9. Gas-sensing response of CeMO30 and CeMO60 when exposed to 0.07 ppm of O 3 as a function of operating temperature.

Fig. 10 .
Fig. 10.Dynamic response-recovery curves of Ce 2 (MoO 4 ) 3 nanocrystals synthesized at different times.(a) CeMO30 and (b) CeMO60 nanopowders exposed to different levels at an operating temperature of 200 C. (c) Comparison of sensor response as a function of ozone concentration.
a and c are lattice parameters, V is the unit cell volume, D hkl is the average crystallite size, and Ɛ hkl is the microstrain.

Table 3
Results of ozone gas-sensing performance of compounds synthesized by different methodologies.